     • date post

16-Apr-2020
• Category

## Documents

• view

0

0

Embed Size (px)

### Transcript of Linear Viscoelasticity manias/MatSE447/Review_2011... Fluid Mechanics Stress Strain Strain rate...

• Fluid Mechanics Stress

Strain

Strain rate

Shear vs. Extension

Apparent Viscosity

Oversimplified Models: Maxwell Model Voigt Model

Continuity Equation

Navier-Stokes Equations

Boundary Conditions

Volumetric Flow Rate

Linear Viscoelasticity Boltzmann Superposition

Step Strain: Relaxation Modulus Generalized Maxwell Model

Viscosity

Creep/Recovery: Creep Compliance Recoverable Compliance

Terminal Relaxation Time

Oscillatory Shear: Storage Modulus Loss Modulus Phase Angle Loss Tangent

Time-Temperature Superposition

1

1

• Molecular Structure Effects

Molecular Models: Rouse Model (Unentangled) Reptation Model (Entangled)

Viscosity

Recoverable Compliance

Diffusion Coefficient

Terminal Relaxation Time

Terminal Modulus

Plateau Modulus

Entanglement Molecular Weight

Glassy Modulus

Transition Zone

Apparent Viscosity

Polydispersity Effects

Branching Effects

Die Swell

2

2

• Nonlinear Viscoelasticity

Stress is an Odd Function of Strain and Strain Rate

Viscosity and Normal Stress are Even Functions of Strain and Strain Rate

Lodge-Meissner Relation

Nonlinear Step Strain Extra Relaxation at Rouse Time Damping Function

Power Law Model Cross Model Carreau Model Cox-Merz Empiricism

First Normal Stress Coefficient

Start-Up and Cessation of Steady Shear

Nonlinear Creep and Recovery

3

3

• Stress and Strain

SHEAR

Shear Stress σ ≡ F A

Shear Strain γ ≡ l h

Shear Rate γ̇ ≡ dγ dt

Hooke’s Law σ = Gγ

Newton’s Law σ = ηγ̇

EXTENSION

Tensile Stress σ ≡ F A

Extensional Strain ε ≡ ∆l l

Extension Rate ε̇ ≡ dε dt

Hooke’s Law σ = 3Gε

Newton’s Law σ = 3ηε̇

1

4

• Viscoelasticity APPARENT VISCOSITY

η ≡ σ γ̇

1.Apparent Viscosity of a Monodisperse Polystyrene.

2

5

• Oversimplified Models MAXWELL MODEL

Stress Relaxation σ(t) = σ0 exp(−t/λ) G(t) = G0 exp(−t/λ)

Creep γ(t) = γ0(1 + t/λ)

J(t) = J0s (1 + t/λ) = J 0 s + t/η

Oscillatory Shear G0(ω) = ωλG”(ω) = G0(ωλ)

2

1 + (ωλ)2

The Maxwell Model is the simplest model of a

VISCOELASTIC LIQUID.

VOIGT MODEL

Creep γ(t) = γ∞[1− exp(−t/λ)] J(t) = J∞[1− exp(−t/λ)]

The Voigt Model is the simplest model of creep for a

VISCOELASTIC SOLID.

3

6

• Equations of Fluid Motion

CONTINUITY

Incompressible ~∇ · ~v = 0 Continuity is a differential equation describing conservation of mass.

NAVIER-STOKES

Slow Flows (no inertia,Re < 1) ρ ∂~v

∂t = −~∇P+ρ~g+η∇2~v

The Navier-Stokes equations are force balances (per unit volume).

DO NOT MEMORIZE CONTINUITY OR N-S EQUATIONS. IF

NEEDED, I WILL GIVE THEM TO YOU.

YOU DO NEED TO KNOW HOW TO USE THEM TO SOLVE

FOR PRESSURE AND VELOCITY DISTRIBUTIONS.

BOUNDARY CONDITIONS

1. NO SLIP at solid surfaces

2. No infinite velocities

MAXIMUM VELOCITY

forvx = vx(y), ∂vx ∂y

= 0

AVERAGE VELOCITY and VOLUMETRIC FLOW RATE

vave = Q

A = 1

A

Z vxdA

4

7

• Linear Viscoelasticity

Stress Relaxation Modulus G(t) ≡ σ(t) γ0

BOLTZMANN SUPERPOSITION: Add effects of many step strains to

construct ANY linear viscoelastic deformation.

Viscosity η0 =

Z ∞ 0

G(t)dt

Creep Compliance J(t) ≡ γ(t) σ

Steady State Compliance J0s = lim t→∞

· J(t)− t

η0

¸ J0s =

1

η20

Z ∞ 0

G(t)tdt

Recoverable Compliance R(t) ≡ γr(t) σ

= J(t)− t η0

J0s = lim t→∞ [R(t)]

Terminal Relaxation Time λ = η0J 0 s =

R∞ 0 G(t)tdtR∞ 0 G(t)dt

5

8

• Linear Viscoelasticity OSCILLATORY SHEAR

apply strain γ(t) = γ0 sin(ωt)

measure stress σ(t) = γ0 [G 0(ω) sin(ωt) +G”(ω) cos(ωt)]

Loss Tangent tan(δ) = G”

G0

Viscosity η0 = lim ω→0

· G”(ω)

ω

¸ Steady State Compliance J0s = lim

ω→0

· G0(ω) [G”(ω)]2

¸

6

9

• Linear Viscoelasticity OSCILLATORY SHEAR RESPONSE

OF A LINEAR MONODISPERSE POLYMER

2.Storage and Loss Modulus Master Curves for Polybutadiene at Refer- ence TemperatureT0 = 25

oC .

7

10

• Linear Viscoelasticity EFFECTS OF MOLECULAR STRUCTURE

6.Storage and Loss Moduli for PolystyreneL15 with Mw = 215000.

11

11

• Linear Viscoelasticity EFFECTS OF MOLECULAR STRUCTURE

7.Storage and Loss Moduli for Polystyrene with Mw = 315000 andMw/Mn = 1.8.

12

12

• MOLECULAR THEORIES

ROUSE MODEL:

DR ∼ 1 N

λR ∼= R 2

DR ∼ N2 G(λR) = ρRT

M η ∼= λRG(λR) ∼ N

G(t) ∼ t1/2 for λN < t < λR REPTATION MODEL: Relaxation is simple Rouse motion up to the Rouse relaxation

time of an entanglement strand.

λe ∼ N2e G(t) ∼ t1/2 for λN < t < λe

Plateau Modulus G0N = ρRT

Me

λd ∼= L 2

DR ∼ N3 D ∼= R

2

λd ∼ 1 N2

η ∼= λdG0N ∼ N3

1

13

• Linear Viscoelasticity TIME-TEMPERATURE SUPERPOSITION

Figure 1: (A) Isothermal Storage Modulus G0(ω) of a Polystyrene at Six Temperatures. (B) Storage Modulus Master Curve at Reference Temperature T0 = 150 0C.

2

14

• Nonlinear Stresses Shear Stress is an odd function of shear strain and shear rate.

σ(γ) = Gγ +A1γ 3 + · · · · ··

σ(γ̇) = η0γ̇ +A2γ̇ 3 + · · · · ··

Apparent viscosity is thus an even function of shear rate.

η(γ̇) ≡ σ(γ̇) γ̇

= η0 +A2γ̇ 2 + · · · · ··

The first normal stress difference is an even function of shear strain and shear rate.

N1(γ) = Gγ 2 +B1γ

4 + · · · · ··

The first term comes from the Lodge-Meissner Relation

N1 σ = γ

N1(γ̇) = Ψ 0 1γ̇ 2 +B2γ̇

4 + · · · · ··

First Normal Stress Coefficient is thus an even function of shear rate.

Ψ1 ≡ N1(γ̇) γ̇2

= Ψ01 +B2γ̇ 2 + · · · · ··

4

15

• Nonlinear Step Strain SHORT-TIME RELAXATION PROCESSES

Figure 3: Nonlinear Relaxation Modulus G(t) for a 6% Polystyrene Solution at 30 oC.

SEPARABILITY AT LONG TIMES

G(t, γ) = h(γ)G(t, 0)

N1(t, γ) = γ 2h(γ)G(t, 0)

h(γ) ≤ 1

5

16

Apparent Viscosity η ≡ σ γ̇

First Normal Stress Coefficient Ψ1 ≡ N1 γ̇2

Figure 4: Shear Rate Dependence of Viscosity and First Normal Stress Coefficient for Low Density Polyethylene.

6

17

• Steady Shear APPARENT VISCOSITY MODELS

Power Law Model η = η0 |λγ̇|n−1

Cross Model η = η0 h 1 + |λγ̇|1−n

i−1

Carreau Model η = η0 h 1 + (λγ̇)2

i(n−1)/2

MOLECULARWEIGHT DEPENDENCES

η0 = KM 3.4 w

λ = η0 G0N ∼M3.4w

Ψ1,0 = 2η 2 0J

0 s ∼M6.8w

THE COX-MERZ EMPIRICISM

η(γ̇) = |η∗(ω)| (ω = γ̇)

7

18

• Nonlinear Viscoelasticity START-UP OF STEADY SHEAR

Figure 5: Shear Stress Growth and Normal Stress Growth Coeffi- cients for the Start-Up of Steady Shear of a Polystyrene Solution.

Start-up of nonlinear steady shear shows maxima in shear and normal stress growth functions, indicating extra short-time relaxation processes induced by the large shear rate.

8

19

• Nonlinear Viscoelasticity CESSATION OF STEADY SHEAR

Figure 6: Shear Stress Decay and Normal Stress Decay Coeffi- cients for Cessation of Steady Shear Flow of a Polyisobutylene Solution.

Shear and normal stresses both decay FASTER at larger shear rates, consistent with long relaxation modes being replaced by shorter-time relaxation processes that are activated in steady shear.

9

20

• Nonlinear Viscoelasticity NONLINEAR CREEP

Figure 7: Creep Compliance at a Linear Viscoelastic Stress σ1 and two Nonlinear Stresses with σ3 > σ2 > σ1.

As stress increases, the viscosity drops and the recoverable strain drops, consistent with large stresses inducing additional dissipation mechanisms.

NONLINEAR RECOVERY

Figure 8: Recoverable Compliance after Creep at Three Stress Levels (Increasing Creep Stress from Top to Bottom).

10

21

• Rheometry

Couette Devices: Gap Loading vs. Surface Loading Controlled Stress vs. Controlled Strain Transducer (and Instrument) Compliance Cone & Plate Parallel Plate Eccentric Rotating Disks Concentric Cylinder Sliding Plates

Poiseuille Devices: Pressure Driven vs. Rate Driven Capilla